Effect of surface chemistry on bacterial adhesion, viability, andmorphology
Paula Parreira,1,2 Ana Magalhaes,3 Ines C. Goncalves,1 Joana Gomes,3 Ricardo Vidal,1
Celso A. Reis,3,4 Deborah E. Leckband,5 M. Cristina L. Martins1
1INEBInstituto de Engenharia Biomedica, Universidade do Porto, Rua do Campo Alegre, 823, 4150-180 Porto, Portugal2Universidade do Porto, Faculdade de Engenharia, Porto, Portugal3IPATIMUPInstituto de Patologia e Imunologia Molecular da Universidade do Porto, Porto, Portugal4Universidade do Porto, Faculdade de Medicina, Porto, Portugal5Department of Chemical and Biomolecular Engineering, University of Illinois at Urbana-Champaign, Urbana, Illinois
Received 21 October 2010; accepted 13 May 2011
Published online 23 August 2011 in Wiley Online Library (wileyonlinelibrary.com). DOI: 10.1002/jbm.a.33178
Abstract: Helicobacter pylori (H. pylori) is one of the most
common infectious agents in the world and it is thought to
colonize the gastric mucosa of about half of the worlds
population causing several gastric diseases. In this work, the
effect of surface chemistry on H. pylori nonspecic adhesion,
viability, and morphology was evaluated using three H. pylori
strains with different adhesins expression prole. Self-
assembled monolayers (SAMs) of alkanethiols on gold were
used to obtain surfaces exposing different functional groups:
OH, CH3, and ethylene glycol (EG4). Bacterial adhesion onto
the surfaces reached a plateau at 2 h. There was a correlation
between adhesion and the exposed surface group, with
bacterial cells adhering preferentially to CH3-SAMs while
EG4-SAMs prevented H. pylori adhesion during the entire
adhesion test (24 h). Surfaces that presented the EG4 group
were also the only ones that signicantly reduced the viabil-
ity of adhered bacteria. Surface chemistry also inuenced
the morphology of adhered bacteria. The H. pylori rod
shape observed in the control (Tissue Culture Polyethylene
TCPE) was only retrieved on CH3-SAMs. This work demon-
strates that surface chemistry, namely specic functional
groups on the material, inuence the nonspecic adsorp-
tion of H. pylori. Moreover, the features of the bacterial
strain and the surface chemistry can alter the adhesion
kinetics, as well as the morphology and viability of
attached bacteria. VC 2011 Wiley Periodicals, Inc. J Biomed Mater
Res Part A: 99A: 344353, 2011.
Key Words: bacterial adhesion, self-assembled monolayers,
SAMs, nanostructured surfaces, Helicobacter pylori, biomaterials
How to cite this article: Parreira P, Magalhaes A, Goncalves IC, Gomes J, Vidal R, Reis CA, Leckband DE, Martins MCL. 2011. Effectof surface chemistry on bacterial adhesion, viability, and morphology. J Biomed Mater Res Part A 2011:99A:344353.
Helicobacter pylori (H. pylori) is a spiral shaped Gram nega-tive bacterium, which colonizes the gastric mucosa, and wasdiscovered by Marshall and Warren.1,2
H. pylori infection has an estimated prevalence of abouthalf the worlds population3, making this pathogen one ofthe most successful human pathogens. Infection by this bac-terium has been associated with increased risk for the de-velopment of gastritis, peptic ulcer disease and gastricadenocarcinomas4. Since 1994, H. pylori is classied by theInternational Agency for Research on Cancer as a class Icarcinogenic agent.
In the last years, an increase in antimicrobial resistancehas led to the partial failure of standard therapeutic treat-ments with antibiotics. This is mainly due to high frequencyof resistant bacteria, which differs between countries, and
according to the H. pylori strain.5,6 Alternative treatmentsmust be developed to counteract the problems faced whentreating infection by this pathogen.
The adhesion of the bacteria to the gastric mucosa is akey step in the establishment of a successful infection. Glycanstructures expressed by the gastric epithelial cells, includingfucosylated ABO blood group antigens7,8 and glycans carryingcharged groups such as sialic acid9, have been identied asreceptors for the bacterial adhesins. Among the large spec-trum of H. pylori putative adhesins, the receptor specicitieshave been described for two adhesins. The blood group anti-gen binding adhesin (BabA) binds to H type-1 and Lewis bantigens, while the sialic acid binding adhesin (SabA) recog-nizes the sialyl-Lewis a and sialyl-Lewis x antigens.9,10 Con-sidering the crucial role of carbohydrate-mediated H. pyloriadhesion in infection, the development of alternative
Correspondence to: M. Cristina L. Martins; e-mail: email@example.com
Contract grant sponsor: Portuguese Foundation for Science and Technology (FCT); contract grant numbers PTDC/CTM/65330/2006, SFRH/BD/
39931/2007, SFRH/BD/36339/2007, SFRH/BD/40563/2007, SFRH/BPD/63722/2009
Contract grant sponsor: NSF; contract grant number DMR 08735
344 VC 2011 WILEY PERIODICALS, INC.
strategies for inhibiting adhesion is an attractive therapeuticapproach.
Studies of nonspecic H. pylori adhesion to syntheticmaterials, such as polypropylene and stainless steel11,12
have been reported. However, very little is known regardingthe effect of different surface chemistry on H. pylori adhe-sion, viability, and morphology. This study evaluated theeffects of surface chemistry, using self-assembled mono-layers (SAMs), which provide an effective approach to con-trol the surface chemistry of a material at the molecularlevel13. Particularly, alkanethiols self assemble into orderedarrays on gold lms, and the x-terminal groups determinethe interfacial properties of the monolayers. Several studieswith proteins and cells have demonstrated the utility ofusing SAMs of long alkanethiols on gold.1417 The effect ofthe surface chemistry on the adhesion of other bacteria,namely Pseudomonas sp18, Staphylococcus epidermidis19,20
and S. aureus21 and Escherichia coli22 have been widelystudied using SAMs.
In this study self-assembled monolayers were used toevaluate the effect of dened surface chemistries, includinghydrophobic CH3-SAMs, hydrophilic OH-SAMs and typicallynon-fouling and protein resistant EG4-SAMs, on the bacterialadhesion kinetics, as well as on the viability and morphol-ogy of H. pylori strains with different expression proles forspecic adhesins.
Self-assembled monolayers (SAMs)Gold substrates were prepared as described previously byour group.14 Briey, a 5-nm chromium adhesion layer and a25-nm gold layer were deposited by ion beam sputteringfrom chromium and gold targets (99.9% purity) on siliconwafers (AUREL, Gmbh). The thin layer of chromiumimproves adhesion of gold to silicon. Just before used, goldsubstrates were cleaned with piranha solution (sevenparts of H2SO4 and three parts of 30% H2O2) for 5 min(caution: this solution reacts violently with many organicmaterials and should be handled with care), thoroughlyrinsed with ethanol, and dried with a gentle argon stream.After cleaning, gold substrates were immersed in thealkanethiol solutions prepared in ethanol (Merck, 99.8%).The 1-mercapto-11-undecyl tetra (ethylene glycol)(SHA(CH2)11AOA(CH2ACH2AO)4AH; EG4; Asemblon,99%), 1-hexadecanethiol (SHA(CH2)15CH3; CH3; Aldrich,92%;) and 11-mercapto-1-undecanol (SH-(CH2)11OH; OH;Aldrich, 97%;) were used as received, in order to preparealkanethiol solutions with a concentration of 0.1 mM forEG4-thiol and 1 mM for CH3- and OH-thiols.
The thiol self-assembly was carried out at room temper-ature for 24 h in a nitrogen environment. The SAMs werethen washed in fresh ethanol, dried with a gentle stream ofpure argon, and then maintained in an argon environmentuntil use.
Bacterial strainsThe H. pylori strains 17875/Leb, 17875babA1::kan babA2::cam(17875babA1A2) and J99 were obtained from the Department
of Medical Biochemistry and Biophysics, Umea University,Sweden. These H. pylori strains have been previouslycharacterized regarding BabA and SabA expression.810,23
The 17875/Leb and J99 strains express both BabA and SabAadhesins while the 17875babA1A2mutant strain only expressesthe SabA adhesin. The H. pylori 17875/Leb although expressingboth adhesins is a spontaneous mutant unable to bind tosialylated antigens.9
Bacterial culture and growth curveH. pylori strains were routinely cultured in Trypticase SoyAgar plates supplemented with 5% sheep blood (BioMer-ieux), in a microaerophilic environment at 37C for 48 h.Afterward, some colonies were transferred to Pylori Agarplates (BioMerieux) and incubated for 24 h under identicalconditions.
For each strain, growth curves were performed in threeindependent experiments. Colonies from Pylori Agar plateswere harvested with liquid medium composed of BHI (BrainHeart Infusion; Oxoid) with an antibiotic cocktail of Poly-mixine B, Vancomycin, Anphotericin B and Trimethroprim(Sigma) and supplemented with inactivated Fetal Bovine Se-rum (Lonza). The initial optical density of each bacteriastrain was adjusted to 0.1 in the referred media (k 600nm) (Shimadzu UV-1201). T-asks containing media andbacterial inoculums were incubated with agitation (150rpm) at 37C under microaerobic conditions in an anaerobicjar with a carbon dioxide generator without catalyst. At dif-ferent time points samples were taken and optical densitywas measured at k 600 nm.
To correlate the values obtained when performing theculture in liquid media versus solid media, colony-formingunits (CFU) were counted in Pylori Agar plates at differenttime points for both culture conditions. Bacteria were har-vested from solid and liquid media at different time points,serial dilutions were done (102 until 107) and 10 lL ofeach dilution plated in Pylori Agar. Incubation was done aspreviously referred. The number of colonies was determinedafter 72 h.
Bacterial adhesionBacteria were harvested from Pylori Agar plates with sterilePBS (phosphate buffer saline; pH 7.4; Sigma). Before incuba-tion with H. pylori strains, the SAMs (EG4A; OHA; CH3-SAMs) and bare gold were hydrated with sterile PBS for15 min. Bacterial suspensions with an optical density of0.080 were mixed with PBS in the wells to achieve a naloptical density of 0,040 (107 cfu mL1). Bacterial concen-tration was selected based on previous work by Azevedoet al.11 Incubation of bacteria with the surfaces was done at37C, and plates were agitated at 120 rpm for 5 min,10 min, 15 min, 30 min, 1 h, 2 h, 6 h, 12 h, and 24 h. Afterincubation, SAMs were rinsed three times with PBS toremove non-adherent bacteria and then xed with 4% (v/v)p-formaldehyde. Bacteria were labeled with 10 lg mL1
DAPI (40,6-diamidino-2-phenylindole dihydrochloride;Sigma) for 30 min and mounted with VectashieldVR Mount-ing Medium (Vector Laboratories). Adherent bacteria were
JOURNAL OF BIOMEDICAL MATERIALS RESEARCH A | 1 DEC 2011 VOL 99A, ISSUE 3 345
visualized with an inverted uorescence microscope (ZeissAxiovert 200 MOT), at 630 magnication. Bacterial countswere performed based on photographs from six randomelds per sample (Area 35272.18 lm2) and wereexpressed as number of bacteria m2. Results are represen-tative of three independent assays using four replicates foreach condition.
Bacterial viabilityThe viability of surface-attached bacteria was accessed usingBacLight Kit (Invitrogen). SAMs and TCPE (Tissue CulturePolyethylene, Sarstedt) were incubated with each H. pyloristrain, with the same optical density as described for bacte-rial adhesion assays. The incubation was for 2 h at 120 rpmand 37C. After incubation, samples were rinsed three timeswith sterile PBS and the procedure was continued accordingBacLight Kit manufacters protocol (Invitrogen). Bacteriawere visualized with an Inverted Fluorescence Microscope,under 400 magnication, and were counted in fourrandom elds per sample. For each strain and surface fourreplicate samples were counted.
Bacterial morphology (scanning electron microscopy)Bacterial morphology was imaged after adhesion onto gold,TCPE and SAMs by Scanning Electron Microscope (SEM;JEOL JSM-6310F), at magnications of 5000 and 20,000.Bacteria were incubated with SAMs as previously describedfor 5 min, 15 min, 30 min, 1 h, and 2 h. After incubation,the samples were rinsed three times with sterile PBS, xedwith 1.5%(v/v) glutaraldehyde (Merck) in 0.14M sodiumcacodylate (Merck), dehydrated with an increasing ethanol/water gradient (50% v/v to 99% v/v), and then subjectedto critical point drying (CPD 7501, Polaron). TCPE sampleswere coated with a gold/palladium lm over 100 s.
H. pylori contact angle measurementsThe water contact angle of the different H. pylori strainswas determined using a contact angle measuring systemfrom Data Physics, model OCA 15, equipped with a elec-tronic syringe, a video CCD-camera and SCA 20 software.The contact angle measurements were performed at roomtemperature (25C) using the sessile drop method withMilli-Q (Millipore) water. Briey, bacteria were cultured asdescribed above and were harvested from Pylori Gelosewith sterile PBS. Measurements were performed on bacte-rial layers deposited on membrane lters according to themethod described by Busscher et al.24 Since the dehydrationof the lters in air, was expected to inuence the results,water contact angles were measured after 20 min of dryingtime. Results were expressed as average values of fourmeasurements.
Zeta potential determinationH. pylori. The zeta potential of different H. pylori strainswas determined using a Zetasizer Nano ZS (Malvern Instru-ments, UK) equipped with a 4 mW HeNe laser beam with awavelength of 633 nm and a scattering angle of 173.Bacteria were cultured as previously described and were
harvested from Petri plates with sterile PBS and used in aconcentration of 107 cfu mL1. Measurements wereperformed in PBS at 37C in polycarbonate folded capillarycells incorporated with gold plated electrodes (DTS1060C).Data were analyzed with the Auto-mode analysis model.The zeta potentials were automatically calculated using theHenry equation with the Smoluchowski approximation. Val-ues are reported as averages based on three individualmeasurements. The results were further corrected to PBS asthe dispersant agent, using the Software DTS Nano v.6.20 toestimate the viscosity, dielectrical constant, and refractionindex from water.
SAMsZeta potentials of SAMs were determined from streamingpotential measurements with a commercial electrokineticanalyzer (EKA) (Anton Paar GmbH, Austria) using a specialrectangular cell for small at samples, with a variable chan-nel height as previously described.25
Two samples (1 1 cm2) were glued on each poly-methyl methacrylate (PMMA) block and mounted in parallelon each side of the cell creating a rectangular (2 1 cm2)slit channel between the sample surfaces. The height of theslit channel was maintained for all the measurements usinga micrometer screw. The Streaming potential was measuredusing Ag/AgCl electrodes installed at both ends of thestreaming channel. The electrolyte used was 1 mM KCl(Sigma-Aldrich) with the pH of 7.4 6 0.1. Experiments wereperformed at 25C. The conductivity of the electrolyte solutionwas measured during the assay. The streaming potential wasmeasured while applying an electrolyte ow in alternatingdirections and pressure ramps from 0 to 400 mbar. For eachsurface, six pressure ramps were performed (three in eachow direction) and in triplicate. The Smoluchowski model wasapplied for zeta potential determination.
Atomic force microscopy (AFM)AFM measurements of SAMs were performed using an Agi-lent 5500 PicoPlus scanning probe microscope. Each samplewas imaged with a 10 10 lm2 piezoscanner. ImageAcquisition was done using Tapping ModeVR , in air and atroom temperature (25C). A silicon nitride cantilever FORTmodel (AppNano, USA) was used with a spring constant of15 N m1 (according to the manufacture information).Images and the surface roughness (Sa) were obtained fromscanned areas of 2500 2500 nm2 on three randomlychosen locations for each sample. Results were expressed asRoughness average (Sa), which was calculated using theWSxM v5.0 software.26
StatisticsThe experimental results were presented as mean valuesand standard deviations. The signicance of differencesbetween mean values was assessed using a one-way ANOVAor independent T sample test (SPSS Software). Signicancewas dened at p < 0.05. Mann-Whitney test was applied toanalyze bacterial water contact angle, bacterial Zeta Poten-tial and AFM results.
346 PARREIRA ET AL. EFFECT OF SURFACE CHEMISTRY ON BACTERIAL ADHESION, VIABILITY, AND MORPHOLOGY
Bacterial growth curveGrowth curves were obtained for the three H. pylori strainsused in these experiments. Different phases that compose agrowth curve, latency (1), exponential growth (2), stationary(3), and death (4), are illustrated in Figure 1.
H. pylori J99 showed a higher growth compared to theother two strains. Both H. pylori 17875/Leb and 17875babA1A2 behaved similarly. H. pylori growth curves wereobtained with cells in liquid medium (BHI Fetal Bovine Se-rum antibiotic cocktail). Figure 2 shows the same growthtendency in both liquid and solid media for all the H. pyloristrains used.
The number of viable bacteria (CFUs) after 12 and 24 his similar for the three strains when bacteria were grown in
solid media. Considering growth in liquid media, there weresome differences in the number of CFUs, namely for J99strain, which presented a lower CFU number. Adhesion testswere performed with bacteria grown from solid mediumwith inocula of 107 cfu ml1 (OD 0.04).
Kinetics of bacterial adhesion to SAMsThe kinetics of H. pylori adhesion to gold and SAMs areillustrated in Figure 3(af). The kinetics of adhesion wasevaluated for the adhesion of the three bacteria strains (J99,17875/Leb, and 17875 babA1A2) to the different surfacesfor up to 24 h. The surface coatings used and their proper-ties have been previously described.15,16,27 These substrateshad different wetabilities, ranging from more hydrophilicOH-SAMs to more hydrophobic CH3-SAMs, as described atTable I.
Regardless of the H. pylori strain used, adhesion ontoEG4-SAMs was extremely low at all times up to 24 h, in ac-cordance with the general non-fouling nature of EG4-SAMs.17,22,28
The initial rate of adhesion of the J99 strain to baregold, OHA and CH3-SAMs prior to plateauing at 2 h, is fast[Fig. 3(b)]. After 2 h, cell adhesion was unchanged for atleast 24 h [Fig. 3(a)].
The adhesion kinetics of the 17875/Leb strain to baregold, OHA and CH3-SAMs was similar to the J99 strain, anddemonstrated a rapid increase up to a plateau at 2 h [Fig.3(d)]. However, at 12 h, there was a decrease of bacterialadhesion on bare gold and on OH-SAMs. The number of
FIGURE 1. Bacterial growth curve of H. pylori J99, H. pylori 17875/Leb
and H. pylori 17875 babA1A2. (1) Latency; (2) Exponential Growth; (3)
Stationary; (4) Death.
FIGURE 2. Correlation between: optical density and CFU in liquid and solid media. (a) H. pylori J99; (b) H. pylori 17875/Leb; (c) H. pylori 17875
JOURNAL OF BIOMEDICAL MATERIALS RESEARCH A | 1 DEC 2011 VOL 99A, ISSUE 3 347
cells attached to CH3-SAMs remained stable until the end ofthe assay (24 h) [Fig. 3(c)].
The kinetics of adhesion of the 17875 babA1A2 strain tobare gold, OH and CH3-SAMs differed from the other twostrains studied, because the number of attached bacteriaplateaued after 2 h only on OH-SAMs [Fig. 3(e)]. The num-ber of attached bacteria on bare gold after 2 h decreased,whereas the number attached to CH3-SAMs continued toincrease until the end of the assay at 24 h. Nevertheless,during the rst 2 h, the adhesion kinetics of H. pylori 17875babA1A2 was similar with the other H. pylori strains used[Fig. 3(f)].
The number of bacteria attached for all three strains ofH. pylori to bare gold (control surface) and model surfaces(SAMs) at 2 h is shown in Figure 4. Adhesion to EG4-SAMswas very low for all bacterial strains used. With exceptionof the 17875/Leb strain, bacterial adhesion was higher onCH3-SAMs. The number of attached 17875/Leb bacteria washigher on gold and on OH-SAMs, followed by CH3-SAMs,and nally EG4-SAMs.
The 17875 babA1A2 strain was the only strain thatexhibited different adhesion levels at 2 h to all of the surfacestested compared to gold (p 0.05) with the number of attachedcells decreasing in the following order: CH3>OH>AuEG4.
FIGURE 3. Adhesion kinetics of H. pylori to SAMs and gold. (a) H. pylori J99 adhesion kinetics up to 24 h; (b) H. pylori J99 adhesion kinetics
until 2 h; (c) H. pylori 17875/Leb adhesion kinetics up to 24 h; (d) H. pylori 17875/Leb adhesion kinetics until 2 h; (e) H. pylori 17875 babA1A2 ad-
hesion kinetics up to 24 h; (f) H. pylori 17875 babA1A2 adhesion kinetics until 2 h.
348 PARREIRA ET AL. EFFECT OF SURFACE CHEMISTRY ON BACTERIAL ADHESION, VIABILITY, AND MORPHOLOGY
Bacterial viability on SAMsThe comparison of bacterial viability after 2 h of adhesionto model surfaces versus adhesion to TCPE (control surface)is shown in Figure 5. Viability was dened as the numberof live attached bacterial cells to total adhered cells.
The different strains exhibited no statistically signicantdifferences in viability; EG4-SAMs were the only coatingsthat showed a signicant decrease in bacterial viability,when compared with TCPE, which is the control surface.The viability of the attached bacteria decreased from 80%on TCPE to 50% on EG4-SAMs. These results demonstratedthat the viability is retained when bacteria are left in con-tact with the model surfaces for at least 2 h.
Bacterial morphology on SAMsThe inuence of the bacterial adherence to the model surfa-ces (bare gold; EG4-; CH3- OH-SAMs and TCPE) on the cellmorphology was also evaluated. Altering morphology is anadaptive response that occurs in order to overcome stressconditions and to enable survival under adverse conditions.SEM images of bacterial morphology were obtained overtime for the different strains when attached to differentsurfaces.
Figure 6 shows H. pylori J99 strain adhered to differentsurface coatings. The morphologies of all bacterial strains inthe different model surfaces evaluated were similar, so thatthese images are representative of all three H. pylori strainstested.
The different surface coatings did inuence the morphol-ogies of bacteria when they were adhered to the substratesurfaces. On gold, none of the adhered bacteria exhibitedthe typical spiral shape that is characteristic of this patho-gen. For the H. pylori strains tested few bacteria adhered tothe EG4-SAMs. Bacteria adherent to CH3-SAMs exhibitedspiral shapes in co-existence with coccoid H. pylori. On OH-SAMs, attached bacteria were all in coccoid form during theentire range of time. On the control TCPE substrate, bothspiral and coccoid bacterial forms were observed.
H. pylori water contact angle determinationWater contact angles for each H. pylori strain used are givenin Table I. Similar values were obtained for the three strainsused, although there is a lower water contact angle of H.pylori J99 comparing to H. pylori 17875babA1A2 (p 0.05).H. pylori 17875/Leb and H. pylori 17875babA1A2 are bothvariants of the CCUG17875 strain so share the same geneticbackground.810 Therefore, it is not surprising that no differ-ences were observed between these two strains.
Zeta potential determinationRegarding H. pylori strains, as expected, the surface poten-tial for bacterial cells was negative (Table I).2931 No signi-cant differences were observed between the three strainsused in our study.
Table I encloses the average zeta potential of gold andSAMs used in this work. Both gold and SAMs were stable at
TABLE I. Water Contact Angle, Zeta Potential and Surface Roughness Results
Water Contact Angle () Zeta Potential (mV) Roughness (Sa) (nm)
Surface Au 63 6 314 44 6 4 0.65 6 0.10EG4-SAMs 38 6 117 38 6 7* 0.60 6 0.06OH-SAMs 18 6 114 38 6 6* 0.58 6 0.05CH3-SAMs 107 6114 43 6 10 0.76 6 0.28
H. pylori strain J99 50 6 2** 7 6 2 17875/Leb 53 6 3 7 6 1 17875 babA1A2 57 6 4** 7 6 1
* Signicantly different from Au (p < 0.05).
** Signicantly different (p < 0.05).
FIGURE 4. H. pylori adhesion to model surfaces and gold at 2h. #Signicantly different from Au (p 0.05) *Signicantly different (p 0.05).
JOURNAL OF BIOMEDICAL MATERIALS RESEARCH A | 1 DEC 2011 VOL 99A, ISSUE 3 349
the experimental conditions and gave reproducible results.Signicant differences (p < 0.05) were observed betweengold and EG4- and OH-SAMs. Despite the observation ofstatistically signicant differences, values can be consideredclose enough and therefore cannot account for observed dif-ferences in bacterial adhesion to our model surfaces.
Atomic force microscopy (AFM)Surface Roughness average (Sa) of all the surfaces used aregiven in Table I. Statistically signicant differences were notobserved between gold surface and SAMs.
It is well known that bacterial adherence to materials isinuenced by the surface chemical and physical properties.The main objective of this study was to identify surfacechemical properties that impact nonspecic adhesion by H.pylori. Assays were performed on PBS, since if medium wasused, duplication and growth would occur and results interms of adhesion would become difcult to interpret.
Self-assembled monolayers (SAMs) of alkanethiols ongold are convenient and versatile platforms for addressingthis issue. Here, we used hydrophobic CH3-SAMs (watercontact angle (yw > 107), hydrophilic OH-SAMs (yw < 20)and typically nonfouling and protein resistant EG4-SAMs.17,28,32 The differences between these SAMs, regardingsurface charge and roughness, are very low (Table I). SAMsroughness was inuenced by the gold surface that has anaverage surface roughness (Sa) of 0.65 6 0.10 nm. In Figure6, the pattern observed on CH3-SAMs was associated withthe xing process used to prepare samples for SEM (cacodi-late and glutalradehyde) after bacterial adhesion. This isalways observed on hydrophobic SAMs, even with othertype of cells. Also, the pores that can be observed are asmall number of pits with a diameter lower than 100 nmon all of the gold surfaces that results from the sputteringprocess. As expected, the values obtained for the zeta poten-tial are negative due to the inuence of the gold supportlayer, being this described previously.33 The value for EG4-SAMs is lower than the one obtained by Martins et al.34
(24 6 0.9 mV), which can be explained by the differentpH at which data was acquired (5.5), since this parameteraffects the zeta potential.35 The three H. pylori strains usedwere also characterized according to their surface chargeand wettability. No differences were observed between theirsurface charges and obtained values are in accordance withthose reported for other bacteria.36,37 Concerning wettabil-ity, values obtained were fairly similar (Table I), rangingfrom 50 to 57 and cannot explain the differences in bacte-rial adhesion to SAMs. H. pylori demonstrated to be morehydrophobic than, for instance, S. epidermidis ATCC 35984(23),38 Serratia marcescens ATCC 13880 (23)36 or Pseudo-monas aeruginosa ATCC 10145 (24).37 Hydrophobic bacte-ria have also been reported, such as P. aeruginosa #3, witha water contact angle of 13236
FIGURE 5. H. pylori viability on model surfaces at 2 h. #Signicantly
different from TCPE (p 0.05).
FIGURE 6. H. pylori J99 morphology when in contact with bare gold; EG4-; CH3-; OH-SAMs and TCPE, at 5 min and 2 hr adhesion times. Obs: A
small number of pits with a diameter lower than 100 nm were always observed in all samples. The pattern observed on CH3-SAMs was asso-
ciated with the xing and drying process used to prepare samples for SEM after bacterial adhesion.
350 PARREIRA ET AL. EFFECT OF SURFACE CHEMISTRY ON BACTERIAL ADHESION, VIABILITY, AND MORPHOLOGY
Bare gold lms were used as a control in the adhesionassay. As expected accordingly to its nonfouling properties,few bacteria adhered to EG4-SAMs up to 24 h, independentof the H. pylori strain tested. Our ndings showing that thedifferent H. pylori strains did not adhere to EG4-SAMs are inaccordance with previous studies describing similar resist-ance to nonspecic protein17 and bacterial adsorption.3941
These results suggest the potential of using EG4-SAMs toimmobilize different candidate ligands of H. pylori becauseall the observed interactions could be exclusively attributedto the immobilized structures.
Initial bacterial adherence to the surfaces occurred withinthe rst minutes of the assay. Only H. pylori adhesion to EG4-SAMs demonstrated to be statistically lower when comparedto other model surfaces, being this difference observed assoon as adhesion time of 5 min (p < 0.05; ANOVA). The fastbacterial adhesion within the rst minutes is in agreementwith the previously described rapid adhesion of H. pylori to ahuman gastric adenocarcinoma epithelial cell line (AGS cellline) in vitro.42 The number of bacteria adhering to SAMsincreased with time up to a limiting plateau, which wasreached at 2 h as described elsewhere.43 The exception is theadhesion of the 17875babA1A2 strain since adhesion keptrising until the end of the assay (24 h).
The H. pylori strains did exhibit differences in their non-specic adhesion to the CH3- and OH-terminated SAMs. J99and 17875babA1A2 showed greater adhesion to hydropho-bic CH3-SAMs after 2 h. This may be explained qualitativelysince the adhesion energy depends on the surface tensionsof bacteria, substrate, and solvating medium (PBS).39
According to the thermodynamic theory44 for two surfacesto come together, resulting in adhesive molecular interac-tions, adsorbed water must be displaced. If the surface ishighly hydrated, such water displacement is energeticallyunfavorable and may be impossible to overcome by thecounteracting attractive interactions.20 Therefore, increasingsubstrate hydrophobicity favors bacterial adhesion, whichcorresponds to the hydrophobic CH3-SAMs. The oppositeoccurs with hydrophilic surfaces (OH-SAMs). Hydrophilicmaterials are reportedly more resistant to protein adsorp-tion45 and bacterial adhesion39 than hydrophobic materials.
By contrast, after 2 h, adherence by the 17875/Lebstrain was highest on gold (control surface) and on OH-SAMs, followed by CH3 and nally by EG4-SAMs. It is inter-esting that this strain adsorbs preferentially to OH-SAMs. AtpH 7.4 the OH group of the hydrophilic SAMs isuncharged45 although the negative zeta potential of all theSAMs used that are inuenced by the zeta potential of thegold surface While electrostatic binding does not explainthe adhesion of this strain to OH-SAMs, it is possible thatthis is due to hydrogen bonding between the terminal AOHgroups and hydrogen bond acceptors or donors on the bac-terial cell wall that may be more prevalent in this strain.
When bacteria adhered to the surfaces, cell viability wasnot signicantly affected by the surface chemistry, but therewere differences in the cell morphologies. Among all thesurfaces tested, except for EG4-SAMs, attached bacteriaremained viable for as long as 2 h.
According to electron microscopy studies H. pylori canexist in three different forms: a viable spiral form, a coccoidform, and a nonviable degenerative form. Because the stom-ach is the natural habitat of this pathogen, when out of itsoptimum environment, this pathogen would likely bestressed. Formation of coccoid forms has been described tohappen under stress conditions, such as in a low nutrientenvironment.46 In human gastric biopsies the coccoid formhas been found in co-existence with the spiral form whenthe bacteria are attached to severely damaged gastric epi-thelial cells.47 This coccoid form was also identied in 93%of biopsy specimens from patients with H. pylori-associatedadenocarcinoma.48 The signicance of the different morpho-logical stages and their role in pathogenesis are controver-sial. Some authors claim that the coccoid stage represents anonviable form because, following conversion to the coccoidform, the bacteria become non-cultivable and cannot berevived, even when subject to optimum growth conditions.Other reports contend that the coccoid form might reect asurvival strategy under extreme conditions,48,49 since it isstill capable of DNA synthesis47 cell binding, and the induc-tion of cellular changes similar to spiral H. pylori, includingtyrosine phosphorylation of host proteins.42 The coccoidform therefore appears to be alive and metabolically active,despite the inability to culture this form. The morphologicaltransformation always seems to occur when cells are inadverse environments,5054 such as increased oxygen ten-sion, alkaline pH,49,50 increased temperature,55 extendedincubation56 or following treatment with omeprazole57 orantibiotics such as amoxicillin.58,59 Regarding the differentsurfaces evaluated in this study, H. pylori could readilyadhere to TCPE and CH3-SAMs and some of the bacteriaremain in the viable and culturable spiral form, whereas ingold and OH- and EG4-SAMs the adhered bacteria were allin the coccoid form. These morphological differences cannotbe attributed to culture conditions or the use of PBS, sinceall H. pylori strain innocula used for the morphology assaysin this study were from the same plate and were manipu-lated identically. Also, bacterial spiral morphology wasmaintained on TCPE and CH3-SAMs even after 2 h on PBS.
This work reports the adhesion, viability, and morphologyof H. pylori adsorbed to self-assembled alkanethiol mono-layers (SAMs), displaying different functional groups, ongold. Bacterial adhesion increased until 2 h, after whattends to stabilize. Except for 17875/Leb strain, whichadhered more to bare gold, the more hydrophobic surfaceCH3-SAMs, had the highest levels of H. pylori adhesion,while the EG4-SAMs prevented bacterial. Moreover, the EG4-SAMs were the only surface that induced a signicant lossof viability of the few adherent bacterial cells. The typical H.pylori spiral shape was only maintained when bacteria wasincubated onto CH3-SAMs and on the control (TCPE),although after 2-h incubation time, the majority of theadhered bacteria were in coccoid shape.
In conclusion, these investigations with model surfacesdemonstrate that different H. pylori strains do exhibit
JOURNAL OF BIOMEDICAL MATERIALS RESEARCH A | 1 DEC 2011 VOL 99A, ISSUE 3 351
differences in nonspecic adsorption that depend on thesurface chemistry and specic functional groups exposed.The identity of the bacterial strain and the surface chemis-try can alter the adhesion kinetics, as well as the morpholo-gies of the attached bacteria.
This study opens new avenues for the comprehensiveapplication of these or chemically similar materials for novelanti-adhesive strategies for H. pylori treatment.
The authors thank Prof. Thomas Boren for providing H. pyloristrains. They also thank M. Manuela Bras for the AFM studies.SEMwas performed at CEMUP (Centro de Materiais da Univer-sidade do Porto).
REFERENCES1. Marshall BJ, Warren JR. Unidentied curved bacilli in the stom-
ach of patients with gastritis and peptic-ulceration. Lancet 1984;1:
2. Marshall B. Unidentied curved bacilli on gastric epithelium in
active chronic gastritis. Lancet 1983;1:12731275.
3. Atherton JC. The pathogenesis of Helicobacter pylori-induced
gastro-duodenal diseases. Annu Rev Pathol 2006;1:6396.
4. Correa P, Houghton J. Carcinogenesis of Helicobacter pylori. Gas-
5. Megraud F. Basis for the management of drug-resistant Helico-
bacter pylori infection. Drugs 2004;64:18931904.
6. Megraud F. H. pylori antibiotic resistance: Prevalence, impor-
tance, and advances in testing. Gut 2004;53:13741384.
7. Boren T, Falk P, Roth KA, Larson G, Normark S. Attachment of
Helicobacter pylori to human gastric epithelium mediated by
blood group antigens. Science 1993;262:18921895.
8. Aspholm M, Olfat FO, Norden J, Sonden B, Lundberg C, Sjostrom
R, Altraja S, Odenbreit S, Haas R, Wadstrom T, Engstrand L,
Semino-Mora C, Liu H, Dubois A, Teneberg S, Arnqvist A, Boren
T. SabA is the H. pylori hemagglutinin and is polymorphic in
binding to sialylated glycans. Plos Pathog 2006;2:e110.
9. Mahdavi J, Sonden B, Hurtig M, Olfat FO, Forsberg L, Roche N,
Angstrom J, Larsson T, Teneberg S, Karlsson KA, Altraja S, Wad-
strom T, Kersulyte D, Berg DE, Dubois A, Petersson C, Magnus-
son KE, Norberg T, Lindh F, Lundskog BB, Arnqvist A,
Hammarstrom L, Boren T. Helicobacter pylori SabA adhesin in
persistent infection and chronic inammation. Science 2002;297:
10. Ilver D, Arnqvist A, Ogren J, Frick IM, Kersulyte D, Incecik ET,
Berg, DE, Covacci A, Engstrand L, Boren T. Helicobacter pylori
adhesin binding fucosylated histo-blood group antigens revealed
by retagging. Science 1998;279:373377.
11. Azevedo NF, Pinto AR, Reis NM, Vieira MJ, Keevil CW. Shear
stress, temperature, and inoculation concentration inuence the
adhesion of water-stressed Helicobacter pylori to stainless steel
304 and polypropylene. Appl Environ Microbiol 2006;72:
12. Azevedo NF, Pacheco AP, Keevil CW, Vieira MJ. Adhesion of
water stressed Helicobacter pylori to abiotic surfaces. J Appl
13. Love JC, Estroff LA, Kriebel JK, Nuzzo RG, Whitesides GM. Self-
assembled monolayers of thiolates on metals as a form of nano-
technology. Chem Rev 2005;105:11031169.
14. Martins MC, Ratner BD, Barbosa MA. Protein adsorption on mix-
tures of hydroxyl- and methyl-terminated alkanethiols self-
assembled monolayers. J Biomed Mater Res A 2003;67:158171.
15. Goncalves IC, Martins MC, Barbosa MA, Ratner BD. Protein adsorp-
tion on 18-alkyl chains immobilized on hydroxyl-terminated self-
assembled monolayers. Biomaterials 2005;26:38913899.
16. Freitas SC, Barbosa MA, Martins MC. The effect of immobilization
of thrombin inhibitors onto self-assembled monolayers on the
adsorption and activity of thrombin. Biomaterials 2010;31:
17. Goncalves IC, Martins MC, Barbosa MA, Naeemi E, Ratner BD.
Selective protein adsorption modulates platelet adhesion and
activation to oligo(ethylene glycol)-terminated self-assembled
monolayers with C18 ligands. J Biomed Mater Res A 2009;89:
18. Wiencek KM, Fletcher M. Bacterial adhesion to hydroxyl- and
methyl-terminated alkanethiol self-assembled monolayers. J Bac-
19. Anderson JM, Patel JD, Ebert M, Ward R. S-epidermidis biolm
formation: Effects of biomaterial surface chemistry and serum
proteins. J Biomed Mater Res A 2007;80A:742751.
20. Katsikogianni MG, Missirlis YF. Bacterial adhesion onto materials
with specic surface chemistries under ow conditions. J Mater
Sci Mater Med 2010;21:963968.
21. Ostuni E, Chapman RG, Liang MN, Meluleni G, Pier G, Ingber DE,
Whitesides GM. Self-assembled monolayers that resist the
adsorption of proteins and the adhesion of bacterial and mamma-
lian cells. Langmuir 2001;17:63366343.
22. Qian XP, Metallo SJ, Choi IS, Wu HK, Liang MN, Whitesides GM.
Arrays of self-assembled monolayers for studying inhibition of
bacterial adhesion. Anal Chem 2002;74:18051810.
23. Magalhaes A, Gomes J, Ismail MN, Haslam SM, Mendes N,
Osorio H, David L, Le Pendu J, Haas R, Dell A, Boren T, Reis CA.
Fut2-null mice display an altered glycosylation prole and
impaired BabA-mediated Helicobacter pylori adhesion to gastric
mucosa. Glycobiology 2009;19:15251536.
24. Busscher HJ, Weerkamp AH, van der Mei HC, van Pelt AW, de
Jong HP, Arends J. Measurement of the surface free energy of
bacterial cell surfaces and its relevance for adhesion. Appl Envi-
ron Microbiol 1984;48:980983.
25. Werner C, Konig U, Augsburg A, Arnhold C, Korber H, Zimmer-
mann R, Jacobasch HJ. Electrokinetic surface characterization of
biomedical polymersA survey. Colloid Surface A 1999;159:
26. Horcas I, Fernandez R, Gomez-Rodriguez JM, Colchero J, Gomez-
Herrero J, Baro AM. WSXM: A software for scanning probe mi-
croscopy and a tool for nanotechnology. Rev Sci Instrum 2007;78:
27. Rodrigues SN, Goncalves IC, Martins MC, Barbosa MA, Ratner
BD. Fibrinogen adsorption, platelet adhesion and activation on
mixed hydroxyl-/methyl-terminated self-assembled monolayers.
28. Martins MC, Curtin SA, Freitas SC, Salgueiro P, Ratner BD, Bar-
bosa MA. Molecularly designed surfaces for blood dehepariniza-
tion using an immobilized heparin-binding peptide. J Biomed
Mater Res A 2009;88:162173.
29. Loder TC, Liss PS. Control by organic coatings of the surface-
charge of estuarine suspended particles. Limnol Oceanogr 1985;
30. van Loosdrecht MC, Lyklema J, Norde W, Schraa G, Zehnder AJ.
Electrophoretic mobility and hydrophobicity as a measured to
predict the initial steps of bacterial adhesion. Appl Environ Micro-
31. Katsikogianni M, Missirlis YF. Concise review of mechanisms of
bacterial adhesion to biomaterials and of techniques used in esti-
mating bacteriamaterial interactions. Eur Cells Mater 2004;8:
32. Johnston E, Ratner B. Protein adsorption: Friend or Foe? InImmobilized biomolecules in analysis: a pratical approach.L.F.e. Cass T, editor. 1998, Oxford University Press: New Yorkp. 7994.
33. Chan YHM, Schweiss R, Werner C, Grunze M. Electrokinetic char-
acterization of oligo- and poly(ethylene glycol)-terminated self-
assembled monolayers on gold and glass surfaces. Langmuir
34. Martins MC, Ochoa-Mendes V, Ferreira G, Barbosa JN, Curtin SA,
Ratner BD, Barbosa MA. Interactions of leukocytes and platelets
with poly(lysine/leucine) immobilized on tetraethylene glycol-ter-
minated self-assembled monolayers. Acta Biomater 2011;7:
35. Schweiss R, Welzel PB, Werner C, Knoll W. Dissociation of surface
functional groups and preferential adsorption of ions on self-
assembled monolayers assessed by streaming potential and
streaming current measurements. Langmuir 2001;17:43044311.
352 PARREIRA ET AL. EFFECT OF SURFACE CHEMISTRY ON BACTERIAL ADHESION, VIABILITY, AND MORPHOLOGY
36. Bruinsma GM, van der Mei HC, Busscher HJ. Bacterial adhesion
to surface hydrophilic and hydrophobic contact lenses. Biomateri-
37. Emerson RJT, Camesano TA. Nanoscale investigation of patho-
genic microbial adhesion to a biomaterial. Appl Environ Microbiol
38. Katsikogianni M, Amanatides E, Mataras D, Missirlis YF. Staphylo-
coccus epidermidis adhesion to He. He/O-2 plasma treated PET
lms and aged materials: Contributions of surface free energy
and shear rate. Colloid Surface B 2008;65:257268.
39. Tegoulia VA, Cooper SL. Staphylococcus aureus adhesion to self-
assembled monolayers: Effect of surface chemistry and brino-
gen presence. Colloid Surface B 2002;24:217228.
40. Qian X, Metallo SJ, Choi IS, Wu H, Liang MN, Whitesides GM.
Arrays of self-assembled monolayers for studying inhibition of
bacterial adhesion. Anal Chem 2002;74:18051810.
41. Faucheux N, Schweiss R, Lutzow K, Werner C, Groth T. Self-
assembled monolayers with different terminating groups as
model substrates for cell adhesion studies. Biomaterials 2004;25:
42. Segal ED, Falkow S, Tompkins LS. Helicobacter pylori attachment
to gastric cells induces cytoskeletal rearrangements and tyrosine
phosphorylation of host cell proteins. Proc Natl Acad Sci USA
43. An YH, Friedman RJ. Concise review of mechanisms of bacterial
adhesion to biomaterial surfaces. J Biomed Mater Res 1998;43:
44. Morra M, Cassinelli C. Bacterial adhesion to polymer surfaces: A
critical review of surface thermodynamic approaches. J Biomater
Sci Polym Ed 1997;9:5574.
45. Silin VV, Weetall H, Vanderah DJ. SPR studies of the nonspecic
adsorption kinetics of human IgG and BSA on gold surfaces
modied by self-assembled monolayers (SAMs). J Colloid Inter-
face Sci 1997;185:94103.
46. Azevedo NF, Almeida C, Cerqueira L, Dias S, Keevil CW, Vieira
MJ. Coccoid form of Helicobacter pylori as a morphological mani-
festation of cell adaptation to the environment. Appl Environ
47. Cole SP, Cirillo D, Kagnoff MF, Guiney DG, Eckmann L. Coccoid
and spiral Helicobacter pylori differ in their abilities to adhere to
gastric epithelial cells and induce interleukin-8 secretion. Infect
48. Bumann D, Habibi H, Kan B, Schmid M, Goosmann C, Brinkmann
V, Meyer TF, Jungblut PR. Lack of stage-specic proteins in
coccoid Helicobacter pylori cells. Infect Immun 2004;72:
49. Enroth H, Wreiber K, Rigo R, Risberg D, Uribe A, Engstrand L.
In vitro aging of Helicobocter pylori: Changes in morphology,
intracellular composition, and surface properties. Helicobacter 1999;4:
50. Kusters JG, Gerrits MM, Van Strijp JA, Vandenbroucke-Grauls
CM. Coccoid forms of Helicobacter pylori are the morphologic
manifestation of cell death. Infect Immun 1997;65:36723679.
51. Sorberg M, Nilsson M, Hanberger H, Nilsson LE. Morphologic
conversion of Helicobacter pylori from bacillary to coccoid form.
Eur J Clin Microbiol Infect Dis 1996;15:216219.
52. Cellini L, Allocati N, Di Campli E, Dainelli B. Helicobacter pylori: A
ckle germ. Microbiol Immunol 1994;38:2530.
53. Chaput C, Ecobichon C, Cayet N, Girardin SE, Werts C, Guadag-
nini S, Prevost MC, Mengin-Lecreulx D, Labigne A, Boneca IG.
Role of AmiA in the morphological transition of Helicobacter
pylori and in immune escape. Plos Pathog 2006;2:e97.
54. Saito N, Konishi K, Sato F, Kato M, Takeda H, Sugiyama T, Asaka
M. Plural transformation-processes from spiral to coccoid Helico-
bacter pylori and its viability. J Infect 2003;46:4955.
55. Shahamat M, Mai U, Paszko-Kolva C, Kessel M, Colwell RR. Use
of autoradiography to assess viability of Helicobacter pylori in
water. Appl Environ Microbiol 1993;59:12311235.
56. Catrenich CE, Makin KM. Characterization of the morphologic
conversion of Helicobacter pylori from bacillary to coccoid forms.
Scand J Gastroenterol Suppl 1991;181:5864.
57. Reynolds DJ, Penn CW. Characteristics of Helicobacter pylori
growth in a dened medium and determination of its amino acid
requirements. Microbiology 1994;140 (Part 10):26492656.
58. Berry V, Jennings K, Woodnutt G. Bactericidal and morphological
effects of amoxicillin on Helicobacter pylori. Antimicrob Agents
59. Bode G, Mauch F, Malfertheiner P. The coccoid forms of Helico-
bacter pylori. Criteria for their viability. Epidemiol Infect 1993;111:
JOURNAL OF BIOMEDICAL MATERIALS RESEARCH A | 1 DEC 2011 VOL 99A, ISSUE 3 353